Phase Transformation and Capacitance ... Phase Transformation and Capacitance Enhancement of Anodic
Embed Size (px)
Transcript of Phase Transformation and Capacitance ... Phase Transformation and Capacitance Enhancement of Anodic
Instructions for use
Title Phase Transformation and Capacitance Enhancement of Anodic ZrO2-SiO2
Author(s) Koyama, S.; Aoki, Y.; Sakaguchi, N.; Nagata, S.; Habazaki, H.
Citation Journal of the Electrochemical Society, 157(12), C444-C451https://doi.org/10.1149/1.3503592
Issue Date 2010-10-22
Doc URL http://hdl.handle.net/2115/44391
Rights © The Electrochemical Society, Inc. 2010. All rights reserved. Except as provided under U.S. copyright law, this work may not be reproduced, resold, distributed, or modified without the express permission of The Electrochemical Society (ECS). The archival version of this work was published in J. Electrochem. Soc., 157(12), C444-C451 (2010)
File Information JES157-12_C444-C451.pdf
Hokkaido University Collection of Scholarly and Academic Papers : HUSCAP
Phase Transformation and Capacitance Enhancement of Anodic ZrO2–SiO2 S. Koyama,a Y. Aoki,a N. Sakaguchi,b S. Nagata,c and H. Habazakia,*,z
aDivision of Materials Chemistry and bCenter for Advanced Research of Energy and Materials, Faculty of Engineering, Hokkaido University, Sapporo 060-8628, Japan cInstitute for Materials Research, Tohoku University, Sendai 980-8577, Japan
Capacitance enhancement of anodic oxide films on zirconium by adding silicon is reported here with correlation to the phase transformation of the oxide. The anodic oxide film formed on zirconium consists mainly of monoclinic ZrO2, which changes to tetragonal ZrO2 phase on the Zr–5.5 atom % Si. Further increase in the silicon contents to 10 and 16 atom % results in the formation of amorphous oxide up to 30 V, above which two-layered films, comprising an outer crystalline tetragonal-phase oxide layer and an inner amorphous layer, are developed. The relative thickness of the outer crystalline layer to the total film thickness increases with formation voltage. The highest capacitance of the anodic oxide films is obtained on the Zr–10 atom % Si. The changes in capacitance, permittivity and formation ratio of anodic oxide films with alloy composition are discussed with phase transformation and growth process of anodic oxides. © 2010 The Electrochemical Society. �DOI: 10.1149/1.3503592� All rights reserved.
Manuscript submitted August 9, 2010; revised manuscript received September 23, 2010. Published October 22, 2010.
ZrO2 is an important inorganic material for high-temperature ap- plications, due to many useful properties such as high strength and stability at high temperatures, oxide ion conductivity at elevated temperatures and radiation-resistant properties. These features make ZrO2 attractive for oxygen sensors, solid oxide fuel cells, and nuclear materials. Moreover, in recent years, zirconia-based materi- als, including ZrO2–SiO2, have been proposed as a promising high-� gate dielectric material for metal-oxide-semiconductor �MOS� transistors.1-3
Thin films of ZrO2 can be prepared by a range of methods, including physical vapor deposition,4 chemical vapor deposition,5
atomic layer deposition,6 chemical solution deposition,3,7 and anodizing.8,9 Anodizing is the most simple and easiest method to form dielectric oxides, and this has been extensively used to form dielectric oxide films on aluminum and tantalum for electrolytic capacitor applications. Tantalum electrolytic capacitors are widely used in electronics industry, but due to limitation of natural re- sources of tantalum and for high demand of increasing capacitance, alternative abundant materials that form oxides with higher permit- tivity, such as niobium and titanium, have been studied.10-16
Zirconium forms usually crystalline anodic oxide films, in con- trast to the formation of amorphous anodic oxides on a range of valve metals, including aluminum, bismuth, niobium, tantalum and tungsten.17 The crystalline structure of anodic zirconium oxide films is influenced by surface treatments prior to anodizing and electrolyte for anodizing. When magnetron-sputtered zirconium is anodized in ammonium pentaborate electrolyte without pretreatment of the de- posited surface, crystalline oxide films, consisting mainly of mono- clinic ZrO2, are developed.
9 The monoclinic phase of ZrO2 is ther- modynamically the most stable at ambient temperature, but amorphous and high-temperature stable phases of cubic or tetrago- nal ZrO2 are also often found in the anodic oxide films formed on chemically polished zirconium, particularly at low formation voltages.18,19 It is also reported that the film structure is dependent on the electrolyte for anodizing.20,21 Such dependence should be associated with the incorporation of foreign species from pretreat- ment bath or electrolyte for anodizing.
Foreign species can be incorporated also from substrate by alloy- ing of zirconium. Film growth and properties of anodic oxide films are examined for the Zr–Ti alloys with a wide composition range.9,15
In these studies, large enhancement of the capacitance and permit- tivity of the anodic oxide films by incorporation of titanium species has been found. The formation of a high-temperature stable phase of
cubic or tetragonal ZrO2, which possesses higher permittivity com- pared with monoclinic ZrO2,
22-24 attributed to the capacitance en- hancement.
Recently, the authors have examined the growth, structure and dielectric properties of anodic oxide films on Zr–16 atom % Si alloy.25 The alloy forms the anodic oxide films with enhanced ca- pacitance, compared with those on zirconium. The outer part of the anodic film consists of the crystalline tetragonal phase, with the remaining inner layer being still amorphous. Further capacitance enhancement is likely to occur due to optimization of alloy compo- sition and controlled film crystallization. The largely enhanced ca- pacitance by alloying of zirconium with silicon makes the Zr–Si alloys attractive as alternative of tantalum capacitor. In the present study, a systematic study of the structure, composition and capaci- tance of the anodic films on the Zr–Si alloys with several silicon contents has been carried out.
Zirconium and Zr–Si alloy films, �200 nm thick, with various silicon contents were prepared by DC magnetron sputtering on to flat glass substrates and aluminum substrates. Prior to the sputtering, the latter substrates were electropolished and subsequently anodized to provide flat surfaces. The specimens prepared on aluminum sub- strates were used mostly for characterization of the anodic oxide films by transmission electron microscope �TEM� and Rutherford backscattering spectroscopy �RBS�. The target used for the prepara- tion of the alloy films was 99.9% zirconium disk of 100 mm in diameter with selected numbers of 99.999 % silicon plates �7.5 � 7.5 mm� located symmetrically on the erosion region. The zirco- nium disk without silicon plates was used for the preparation of the zirconium films. The silicon contents in the alloy films were deter- mined using TEM-EDX analysis.
The specimens were anodized at several formation voltages up to 100 V for 900 s in stirred 0.1 mol dm−3 ammonium pentaborate electrolyte at 298 K, using a two-electrode cell with a platinum counter electrode. Initially, a constant current density of 50 A m−2
was applied to reach the selected formation voltage. Electrochemical impedance measurements were carried out in the same electrolyte by applying 50 mV �rms� of sinusoidal alternating voltage in the 100 to 104 Hz range, and the capacitances of the anodic oxide films were determined by analyzing the Bode diagrams.
Vertical cross sections of the anodic oxide films were observed using a TEM �JEOL JEM-2000FX� operating at a voltage of 200 kV. High-resolution transmission electron microscopy �HR- TEM� of the films was carried out using a FEG-TEM �JEOL JEM- 2010F� operating at a voltage of 200 kV. Electron transparent sec- tions, about 30 nm thick, were generated using an ultramicrotome
* Electrochemical Society Active Member. z E-mail: email@example.com
Journal of The Electrochemical Society, 157 �12� C444-C451 �2010� 0013-4651/2010/157�12�/C444/8/$28.00 © The Electrochemical Society
Downloaded 06 Dec 2010 to 220.127.116.11. Redistribution subject to ECS license or copyright; see http://www.ecsdl.org/terms_use.jsp
�Reichert-Nissei Ultracut S� with a diamond knife. The structures of the deposited zirconium and Zr–Si alloys, as well as the anodic oxide films, were identified by grazing incidence X-ray diffraction �GIXRD� using Cu K� radiation with the incident angle of 2° �Rigaku, RINT-2000 system�. Raman measurements of anodic oxide films were performed using a 531.9 nm laser with Synapse CCD detector. Laser power at the sample was kept to 6 mW. Composi- tions of anodic oxide films and alloy films were determined by RBS, using a 2.0 MeV He2+ ion beam supplied by a tandem-type accel- erator at Tohoku University. The scattered particles were detected at 170° to the incident beam direction, which was normal to the speci- men surface. The data were analyzed using the RUMP program.
Phases of deposited alloy films.— Figure 1 shows GIXRD pat- terns of the sputter-deposited zirconium and Zr–Si alloys. The pat- tern of the zirconium reveals an hcp structure. The pattern of the Zr–5.5 atom % Si also shows an hcp structure, but only two diffrac- tion lines of 002 and 103 appear, indicating different grain orienta- tions between zirconium and Zr–5.5 atom % Si films. The diffrac- tion lines shift slightly to lower angles by silicon addition, suggestin